The influence of warm forming in natural aging and springback of Al-Mg-Si alloys
- 215 Downloads
Warm forming is a very interesting solution to improve formability and reduce springback. Natural aging is an open issue for heat treatable aluminum alloys, since it causes variability in sheet metal forming operations, namely in the parts shape, as well as in-service behavior. Therefore, this work aims to study the contribution of warm forming to minimize the variability caused by natural aging and reduce the springback in sheet metal forming operations. The thermo-mechanical behavior of two Al-Mg-Si alloys, EN AW 6016-T4 and EN AW 6061-T6, is studied in function of temperature (from 22 to 300 °C) using uniaxial tensile tests, cylindrical cup tests and split ring (springback) tests. Moreover, for the EN AW 6016-T4, the study was also performed in function of the storage time (from 1 to 18 months). At 22 °C, the increase of the storage time leads to a clear increase of the yield stress and of the work hardening and, consequently, of the springback. Warm forming at temperatures between 200 and 250 °C, using a short exposure time, reduces the yield stress and the work hardening and, consequently, springback for both alloys. Moreover, the effect of natural aging is minimized. Thus, warm conditions can be used as an effective solution to minimize the variability caused by the natural aging and reduce the springback in forming operations of heat treatable aluminum alloys.
KeywordsAl-Mg-Si alloys Natural aging Warm forming Springback
The authors would like to acknowledge the funding that sponsored this research work: the national funds from the French Ministry of Higher Education and the Portuguese Foundation for Science and Technology (FCT) via the project P2020-PTDC/EMS-TEC/6400/2014 (POCI-01-0145-FEDER-016876) and by UE/FEDER funds through the program COMPETE 2020, under the project CENTRO-01-0145-FEDER-000014 (MATIS). The first author V. Simões is also grateful to the FCT for the PhD grant SFRH/BD/90669/2012. The authors are also grateful to Constellium (Estelle Muller) for supplying the material. Moreover, the authors acknowledge the technical staff of IRDL, for their help in some of the experimental procedures (Anthony Jégat and Hervé Bellegou).
This study was funded by the French Ministry of Higher Education and the Portuguese Foundation for Science and Technology (FCT) via the project P2020-PTDC/EMS-TEC/6400/2014 (POCI-01-0145-FEDER-016876) and by UE/FEDER funds through the program COMPETE 2020, under the project CENTRO-01-0145-FEDER-000014 (MATIS). The first author V. Simões was also funded by the FCT for the PhD grant SFRH/BD/90669/2012.
Compliance with Ethical Standards
Conflict of Interest
The authors declare that they have no conflict of interest.
- 8.Zhong H, Rometsch P, Cao L et al (2010) Tensile properties and work hardening behaviour of alloy 6016 in naturally aged and pre-aged conditions. In: Proceedings of the 12th international conference on aluminium alloys. Japan Institute of Light Metals, Tokyo, Japan, pp 2203–2208Google Scholar
- 13.Yan Y (2014) Investigation of the negative and positive effect of natural aging on artificial aging response in Al-Mg-Si alloys. PhD-thesis, Technische Universität BerlinGoogle Scholar
- 20.AMAG (2012) AluReport 03/2012 - 7xxx-high strength aluminum sheets for lightweight automotive applications. 6–9Google Scholar
- 22.ISO 6892-1:2009 (2009) Metallic materials - tensile testing - part 1: method of test at room temperature. International Organization for Standardization, GenevaGoogle Scholar
- 23.Kurukuri S (2010) Simulation of thermally assisted forming of aluminium sheet. PhD-thesis, University of TwenteGoogle Scholar
- 24.Kaufman JG (2008) Properties of aluminum alloys: fatigue data and effects of temperature, product form, and processing. ASM International, Materials ParkGoogle Scholar
- 25.The Aluminum Association (2015) International alloy designations and chemical composition limits for wrought aluminum and wrought aluminum alloys. http://www.aluminum.org/sites/default/files/TEAL_1_OL_2015.pdf. Accessed 9 Feb 2017
- 34.Coër J, Laurent H, Oliveira MC et al (2017) Detailed experimental and numerical analysis of a cylindrical cup deep drawing: pros and cons of using solid-shell elements. Int J Mater Form:1–17. https://doi.org/10.1007/s12289-017-1357-4
- 36.Jelt Grease 5411 aerosol 95cSt. http://fr.rs-online.com/web/p/graisses/4612124/. Accessed 25 Nov 2015
- 37.ASTM E2492-07(2012) (2012) Standard test method for evaluating springback of sheet metal using the Demeri split ring test. ASTM Int 03.01. doi: https://doi.org/10.1520/E2492-07R12
- 39.Xia ZC, Miller CE, Ren F (2004) Springback behavior of AA6111-T4 with split-ring test. In: AIP conference proceedings. AIP Publishing, pp 934–939Google Scholar
- 41.Simões VM, Coër J, Laurent H et al (2013) Sensitivity analysis of process parameters in the drawing and ironing processes. Key Eng Mater 554–557:2256–2265. https://doi.org/10.4028/www.scientific.net/KEM.554-557.2256 CrossRefGoogle Scholar
- 48.Simões VM, Oliveira MC, Neto DM et al (2017) Numerical study of springback using the split-ring test: influence of the clearance between the die and the punch. Int J Mater Form:1–13. https://doi.org/10.1007/s12289-017-1351-x